A Layered Hybrid Rare-Earth Double Perovskite with Two Continuous Reversible Phase Transitions Induced By Unusual Two Driving Gears of Fan-Like Rotation Movements
Li, Duo-Fu; Guo, Feng; He, Xiao-Li; Wu, Yao-Zhen; Deng, Xiang-Hong; Yang, Kang-Ping; Sui, Yan; Li, Yongxiu; CrystEngComm  (2022) –; doi:10.1039/D2CE01297A

data_7245742
_publ_section_title
;
 A Layered Hybrid Rare-Earth Double Perovskite with Two Continuous
 Reversible Phase Transitions Induced By Unusual Two Driving Gears of
 Fan-Like Rotation Movements
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/D2CE01297A
_journal_year                    2022
_chemical_formula_moiety         'C28 H56 Eu K N12 O24'
_chemical_formula_sum            'C28 H56 Eu K N12 O24'
_chemical_formula_weight         1135.90
_space_group_crystal_system      orthorhombic
_space_group_IT_number           51
_space_group_name_Hall           '-P 2a 2a'
_space_group_name_H-M_alt        'P m m a'
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2022-10-11 deposited with the CCDC.	2022-10-31 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   23.6915(11)
_cell_length_b                   9.7624(3)
_cell_length_c                   9.9066(4)
_cell_measurement_reflns_used    2605
_cell_measurement_temperature    313(2)
_cell_measurement_theta_max      27.2630
_cell_measurement_theta_min      3.9960
_cell_volume                     2291.26(16)
_computing_cell_refinement       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_collection       'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_data_reduction        'CrysAlisPro 1.171.40.53 (Rigaku OD, 2019)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      313(2)
_diffrn_measured_fraction_theta_full 0.978
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'SuperNova, Single source at offset/far, EosS2'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0227
_diffrn_reflns_av_unetI/netI     0.0302
_diffrn_reflns_Laue_measured_fraction_full 0.978
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            6011
_diffrn_reflns_point_group_measured_fraction_full 0.978
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.027
_diffrn_reflns_theta_min         3.299
_diffrn_source                   'micro-focus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    1.556
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.88984
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.40.53 (Rigaku Oxford Diffraction, 2019)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.646
_exptl_crystal_description       block
_exptl_crystal_F_000             1164
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.200
_exptl_crystal_size_min          0.180
_refine_diff_density_max         1.232
_refine_diff_density_min         -0.879
_refine_diff_density_rms         0.125
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     211
_refine_ls_number_reflns         2215
_refine_ls_number_restraints     40
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0654
_refine_ls_R_factor_gt           0.0549
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0851P)^2^+6.5522P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1426
_refine_ls_wR_factor_ref         0.1523
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1852
_reflns_number_total             2215
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d2ce01297a2.cif
_cod_data_source_block           20211126-LDF-351-313K
_cod_database_code               7245742
_shelx_estimated_absorpt_t_min   0.746
_shelx_estimated_absorpt_t_max   0.767
_shelxl_version_number           2014-3
_shelx_res_checksum              3969
_shelx_hkl_checksum              83064